1

**Effect of electron-phonon interaction on the room ** **temperature thermoelectric properties of bulk MoSe**

^{2}Md Golam Rosul^{1}, Mona Zebarjadi^{1,2,*}

1Department of Electrical and Computer Engineering, University of Virginia, Charlottesville, VA 22904, United States

2Department of Materials Science and Engineering, University of Virginia, Charlottesville, VA 22904, United States

*Corresponding author: mz6g@virginia.edu

**Abstract **

We study the thermoelectric properties of bulk MoSe2 within relaxation time approximation including electron-phonon and ionized impurity interactions using first- principles calculations and at room temperatures. The anisotropy of this two- dimensional layered metal dichalcogenide is studied by calculations of electron mobility in the cross-plane and the in-plane directions. We show that the cross-plane mobility is two orders of magnitude smaller than the in-plane one. The inclusion of van der Waals interactions further lowers the carrier mobility in the cross-plane direction but minimally affects the in-plane one. The results for in-plane electrical mobility and conductivity are in close agreement with experimentally reported values indicating the accuracy of the calculations and the dominance of the electron-phonon scattering rates at low carrier concentrations and the combination of electron-phonon and ionized impurity scattering at high carrier concentrations. The Seebeck coefficient calculations show that this

2 coefficient is primarily dictated by the band structure. The details of relaxation times and inclusion of van der Waals interactions only slightly change the Seebeck coefficient.

**Introduction **

Thermoelectric materials can convert heat energy directly to electricity and vice versa.

Thermoelectric materials are considered to have great potential for power generation,
energy-saving, and heat management [1–6]. Devices made of thermoelectric materials are
extremely simple, have no moving parts, use no greenhouse gases, have a quiet
operation, are environmentally friendly, and are highly reliable [7,8]. Because of these
excellent features, thermoelectric devices have attracted extensive interest for nearly two
centuries. Solid-state thermoelectric devices are generally based on heavily doped
semiconductors such as chalcogenides [9,10], zintl phases [11], clathrates [12], complex
oxides [13], and skutterudites [14,15], and can be used for cooling applications or
electricity generation directly from a heat source. The efficiency of these devices is
*determined by a dimensionless figure-of-merit ZT = (S*^{2}*σ/k)T where Z is the figure-of-*
*merit, T is the absolute temperature, S is the Seebeck coefficient, σ is the electrical *
*conductivity, and k is the total thermal conductivity with contributions from the lattice *
*(k*^{L}*) and the electrons (k*^{e}) [16]. Besides the traditional power generator and cooling
applications, thermoelectric materialscan also be applied to active cooling [17,18], where
large thermal conductivity and power factorare both desired to transfer heat from high-

3 temperature heat sources to low-temperature heat sinks, and in thermal switches where heat flux is required to adjust based on ambient conditions [19].

Two-dimensional (2D) layered materials such as transition metal dichalcogenides (TMDCs) are good candidates for thermoelectric [20–27] as well as thermionic [28–31]

energy conversion applications because of their large Seebeck coefficients and low
thermal conductivities. Due to weak van der Waals interactions, the thermal conductivity
in the cross-plane direction is small making them ideal candidates for nanoscale
cooling [32–34] and power generation. Another important feature of 2D materialsis that
the thermoelectric properties such as electrical conductivity and Seebeck coefficient
depend on the number of layers as the band structure and the bandgap change with it. In
the case of MoSe^{2,} its bulk has an indirect bandgap of 0.80 eV while monolayer MoSe^{2}
has a direct bandgap of 1.55 eV [35–37].

MoSe^{2}, a TMDC material, consists of a transition metal Mo, sandwiched between two
chalcogen layers of Se in which Mo’s and Se’s are covalently bonded within the plane.

However, the Se layer constructs weak van der Waals (vdW) interaction with the next Se layer perpendicular to the plane to construct bulk MoSe2. Therefore, it is important to include the van der Waals interaction in the theoretical calculation to correctly obtain the thermoelectric transport properties of MoSe2. It is expected that the inclusion of vdW interaction in the theoretical calculation affects the cross-plane transport properties significantly.

4 Thermoelectricity in semiconductors is the response of electron and phonon currents to temperature gradients. The interaction between the electrons and phonons plays a crucial role in this response. To maximize the thermoelectric response, one needs to selectively heat electrons and minimize the electron-phonon interaction to avoid heat leakage to the lattice. Only the energy delivered by the electrons is the conversion of heat to electrical energy, the part delivered by phonons is wasted. In practice, phonons always exist at finite temperatures and take some of the input heat directly from the source and some through electron-phonon energy exchange. Both, lower the performance and serve as heat leaks. Electron-phonon interaction is an important phenomenon in condensed matter physics beyond thermoelectricity. Many experimental observations such as temperature-dependent band structures, zero-point renormalization of the bandgap in semiconductors, conventional phonon-mediated superconductivity, phonon-assisted light absorption, Peierls instability [38], the Kohn effect [39], temperature-dependent electrical resistivity as well as traditional superconductivity [40] are caused by the electron-phonon interaction. The role of electron-phonon interactions in the transport properties of systems with strong electron-phonon correlations is one of the central issues in the theory of strongly correlated systems.

Electron-phonon scattering plays a central role in electron transport in relatively pure materials [41]. While the impurity and defects lower the electron mobility, their values are not intrinsic and depend on the quality of the material growth and the number of

5 impurity and defect centers. In contrast, electron-phonon interaction is an intrinsic property of a given semiconductor and hence the first step in evaluating the potential of a semiconductor for thermoelectric applications is to evaluate the electron-phonon interaction. Over the years, several different open-source codes have been developed to compute the electron-phonon scattering rate from first-principles calculations [42–46].

These fully first-principles approaches to calculating the electron-phonon interaction employing density functional perturbation theory (DFPT) combined with Wannier interpolation [47] can now produce highly accurate electron lifetimes and have shown close agreement with experimental measurements of electron mobility and conductivity of intrinsic samples [43,45].

In the case of doped semiconductors, it is important to include ionized impurity scattering in addition to electron-phonon interactions. The carrier density in a doped semiconductor is determined by the relative position of the impurity states to the band edges (the binding energy) and the temperature. When ionized, the charged impurity centers scatter the free carriers via Coulomb interactions, affecting their lifetimes. At low temperatures, when phonon effects are minimal, carrier scattering by ionized impurities is the dominant scattering determining the carrier mobility. In heavily doped semiconductors, this regime might be extended to room temperatures. Therefore, it is important to incorporate ionized impurity scattering along with electron-phonon

6 scattering in the theoretical transport calculation to accurately predict experimental results.

In this work, we theoretically evaluate the effect of electron-phonon scattering (EPS) and
ionized impurity scattering (IIS) on the electronic and thermoelectric properties of bulk
MoSe2 in the in-plane and cross-plane direction at room temperature without and with
including the effect of vdW interaction. We obtain the EPS rates from the first-principle
calculations and the IIS rates using Brooks-Herring [48] approach. The electronic and
*thermoelectric transport properties such as mobility (µ), electrical conductivity (σ), and *
*Seebeck coefficient (S)*ofbulk MoSe2 at room temperature in the in-plane and cross-plane
direction are calculated by solving the linearizedelectron Boltzmann transport equation
(BTE) under the relaxation time approximation (RTA) with the aid of the EPS rates and
IIS rates evaluated at different Fermi Levelpositions. Finally, we compare the calculated
in-plane mobility and electrical conductivity with experimentally obtained values.

**Computational Details **

We compute the EPS rates in bulk MoSe2 using first-principles calculations. The equilibrium properties of electrons and phonons are calculated using the density functional theory (DFT) and density functional perturbation theory (DFPT) as implemented in the QUANTUM ESPRESSO package [49]. The norm-conserving pseudopotentials [50] with the Perdew-Burke-Ernzerhof (PBE) [51] functional for the exchange-correlation are used. We used the non-local van der Waals DFT functional

7
(vdW-DF-optb86) [52,53] to correctly take the vdW interaction into account. A 12×12×4
mesh and an 18×18×6 Monkhorst-Pack k-point mesh are used for the self-consistent and
non-self-consistent field calculations, respectively and the cutoff energy of the plane
wave is chosen as 60 Ry. The convergence threshold of energy is set to be 10^{−12} Ry. Lattice
was relaxed with the force convergence threshold of 1.0e^{-4} Ry/Bohr. Theobtained relaxed
lattice constants of bulk MoSe^{2} in the hexagonal structure are a=b=3.31 Å and c=12.89 Å.

Our calculated lattice constants match the experimentally reported value in the
literature [54]. The dynamical matrices and phonon perturbations are computed on a
6×6×2 q-point mesh in the phonon calculations. To obtain the EPS rates, the PERTURBO
package [45] is employed to interpolate the electron-phonon coupling matrices as well as
electron and phonon eigenvalues obtained by DFT and DFPT calculations from coarse to
fine k and q point meshes (40×40×40) using the Wannier interpolation scheme [55]. The
Wannier function consists of d^{xy}, d^{xz}, d^{yz}, d^{z2}, d^{x2-y2 }orbitals on each Mo atom and p^{x}, p^{y}, p^{z}
orbitals on each Se atom, leading to the wannierization of a total of 22 bands. In addition,
and for comparison and validation, the EPS rates are also computed using the electron-
phonon Wannier (EPW) [43] package based on maximally localized Wannier
functions [55,56], which allows accurate interpolation of electron-phonon couplings from
coarse grids to arbitrarily dense grids. The EPS rates calculated using these two packages
show similar values. We calculated the IIS rates using the Brooks-Herring approach for
different doping concentrations [48]. The IIS rate is given by,

8
𝜏_{𝑖𝑚𝑝}(𝐸) = 8𝜋^{3}ħ^{3}𝜀_{𝑟}^{2}𝜀_{0}^{2}

𝑁_{𝐼}𝑞^{4} [ln(1 + 𝛶^{2}) − 𝛶^{2}
1 + 𝛶^{2}]

−1

𝐷𝑂𝑆(𝐸)𝑣^{2}(𝐸)

where 𝛶^{2} = 4𝜋^{2}𝐿^{2}_{𝐷}ħ𝐷𝑂𝑆(𝐸)𝑣(𝐸), ħ is the reduced Plank constant, 𝜀_{𝑟} is the relative
permittivity, 𝜀_{0} is the permittivity of free space, 𝑁_{𝐼} is the impurity concentration, 𝑞 is the
electronic charge, 𝐿_{𝐷} is the Debye length, 𝐷𝑂𝑆(𝐸) is the density of states, and 𝑣(𝐸) is the
group velocity.

The electron mobilities, electrical conductivities, and the Seebeck coefficients are
**calculated using the PERTURBO [45] code based on the BTE under the RTA. **

**Result and Discussion **

The electronic band structures of bulk MoSe2 with and without the inclusion of vdW interaction are shown in Fig. 1(a). The band structure calculated in this work is in agreement with the previous calculation [57]. The bulk MoSe2 shows an indirect bandgap of 0.80 eV. This is in agreement with the previously reported theoretical value [36,37].

The calculated phonon dispersions using DFPT with and without the inclusion of vdW interaction are shown in Fig. 1(b). The DFT band structure was then interpolated using the maximally localized Wannier function. The DFT calculated band structures and the band structure obtained from Wannier interpolation show very good agreement (see

9 Supplemental Information). We observe that the effect of vdW interactions is minimal on the band structure and the phonon dispersions.

We focus on the n-type samples and study the electron-phonon interaction within the
conduction band. Figure 2 (a) shows the calculated EPS rates obtained from the EPW
and PERTURBO codes together with the electronic density of states (DOS) with respect
to the conduction band minimum (CBM). The EPS rates obtained from these two codes
show close agreement. The scattering rates versus electron energy show a similar trend
to that of the electronic DOS, consistent with the fact that the DOS regulates the phase
space for electron-phonon scattering [58]. The IIS rates for the carrier concentration of
10^{16}, 10^{17}, and 10^{18} cm^{-3} at 300K along with the EPS rates are shown in Fig. 2 (b).

Using our calculated scattering rates, the room-temperature electron mobilities and electrical conductivities are calculated using the BTE under the RTA. In this paper, we mainly focus on electron transport in the in-plane and cross-plane directions at room Figure 1. (a) Electronic band structure and (b) phonon dispersion of bulk MoSe2 without (red) and with (blue) the inclusion of vdW interaction.

10
temperature. The electron transport properties namely the mobility and conductivity are
calculated for four combinations as shown in Figs. 3 and 4: (i) without vdW interaction
and inclusion of only EPS rates (red curves), (ii) with vdW interaction and inclusion of
only EPS rates (blue curves), (iii) without vdW interaction and inclusion of the
combination of EPS and IIS rates (green curves), and (iv) with vdW interaction and
inclusion of the combination of EPS and IIS rates (black curves). Figure 3 shows the room
temperature electron mobility in the in-plane and cross-plane direction for the carrier
concentration range of 10^{16} to 10^{18} cm^{-3}. Our calculated in-plane electron mobility at room
temperature with the inclusion of only EPS rates and without vdW interaction is 192
cm^{2}/Vs while including the vdW interaction is 200 cm^{2}/Vs. These values are independent
of the carrier concentration. The obtained cross-plane mobility with the inclusion of only
EPS rates and without including the vdW interaction is 2.47 cm^{2}/Vs while with including
the vdW interaction is 1.46 cm^{2}/Vs. We can see that the effect of vdW interaction on the
Figure 2. (a) Electron-phonon scattering rates in MoSe^{2} calculated using EPW and PERTURBO
code together with the electronic density of states. (b) Electron-phonon scattering rates and
ionized-impurity scattering rates with carrier concentration between 10^{16} and 10^{18} cm^{-3} at 300 K.

11 in-plane mobility is small while the cross-plane mobility decreased by a factor of 1.7. This is expected as Mo’s and Se’s are covalently bonded within the plane while the Se layer constructs weak vdW interaction with the next Se layer in the cross-plane direction in the MoSe2 structure and to accurately predict the electronic transport in the cross-plane direction this vdW interaction needs to be accounted for in the calculations.

The theoretical mobility with the inclusion of only EPS rate is relatively insensitive to
carrier concentration within the carrier concentration range of 10^{16} to 10^{18} cm^{-3}. The
experimentally measured in-plane room temperature Hall mobilities of single-crystal
MoSe2 are extracted from literature for different carrier concentrations. Within the range
of carrier concentration from 3x10^{16} to 1.4x10^{17} cm^{-3}, the Hall mobility varies from ^{~}55 to

~175 cm^{2}/Vs as shown in Fig 3(a). The calculated in-plane mobility is overestimated
compared to all the experimentally measured values. This is because we only included
the EPS rates in the transport calculation which is the dominant scattering mechanism at
Figure 3. The (a) in-plane and (b) cross-plane mobility vs carrier concentration are calculated
using the Boltzmann transport equation under the constant relaxation time approximation. The
in-plane electrical mobilities are compared with the in-plane experimental Hall mobilities from
**literature. **

12 low carrier concentration. However, as the carrier concentration increases, the contribution of the IIS rates in the transport properties is no longer negligible. Therefore, we need to include both the EPS rates and IIS rates in the transport calculation to correctly predict the experimental results. We can see from Fig. 3 that with the inclusion of both EPS rates and IIS rates in the transport calculation, mobility gradually decreases as the carrier concentration increases in the in-plane and cross-plane direction. Furthermore, we can see from Fig. 3a that the in-plane theoretical mobility closely matches the experimental mobility with the inclusion of both EPS rates and IIS rates thus confirming that the IIS rates need to be accounted for in the transport calculation to accurately predict electronic transport properties.

Next, we calculate the in-plane and cross-plane electrical conductivities at room temperature for the same four combinations. The calculated in-plane and cross-plane

Figure 4. The (a) in-plane and (b) cross-plane electrical conductivity vs carrier concentration is
calculated using the Boltzmann transport equation under the constant relaxation time
approximation. The in-plane electrical conductivity is compared with the electrical conductivity
of single crystal MoSe^{2} from the literature.

13
room temperature electrical conductivity for carrier concentrations from 10^{16} to 10^{18} cm^{-3}
are shown in Fig. 4. First, we calculate the in-plane and cross-plane electrical
conductivities with the inclusion of only EPS rates. The in-plane and cross-plane electrical
conductivities increase as the carrier concentrations increase, which is consistent with the
behavior of semiconductor materials. The inclusion of vdW interaction does not affect the
in-plane electrical conductivity as shown by the overlap of red and blue lines in Fig. 4 (a).

However, the vdW interaction reduces the cross-plane electrical conductivity as shown in Fig. 4 (b). We compare our calculated in-plane electrical conductivity with the experimentally measured in-plane electrical conductivity of single crystal MoSe2 [59–62].

Our calculated in-plane values are larger than the experimental values as shown in Fig.

4(a). This is consistent with the fact that other scattering mechanisms are present in real materials along with EPS whereas we only included the EPS rates in the transport calculation. Therefore, we included the combination of both EPS rate and IIS rate in the transport calculation. We can see from Fig. 4 that the inclusion of IIS rates along with EPS rates has a small effect on the electrical conductivity at low carrier concentration but significantly modifies it as the carrier concentration becomes large. Now, our calculated in-plane electrical conductivity values closely match the experimental values as shown in Fig. 4(a) implying that the inclusion of both the EPS rate and IIS rate is important in the transport calculation of bulk MoSe2 at room temperature.

14 The in-plane and cross-plane Seebeck coefficients are calculated using the BTE under the RTA. In this case, only the theoretically calculated EPS rates from the first principles are used to estimate the relaxation time. To carry out the quantitative comparison, we calculate the Seebeck coefficient using the constant relaxation time approximation (CRTA) employing the BoltzTrap code [63]. Figures 5 (a) and 5(b) show the room temperature in-plane and cross-plane Seebeck coefficient vs chemical potential with respect to the conduction band minimum (CBM) calculated using RTA and CRTA. The Seebeck coefficient from RTA and CRTA show very good agreement confirming that the Seebeck coefficient is not sensitive to the details of relaxation times. The calculated Seebeck coefficients with and without including the vdW interaction are also shown in Fig. 5. The Seebeck coefficient value decreases as the chemical potential increases, which is consistent with the fact that higher chemical potential represents higher carrier

Figure 5. Room temperature Seebeck coefficient vs chemical potential in the (a) in-plane and (b) cross-plane direction. The conduction band minima calculated from Boltztrap and Perturbo code is taken as the reference point, zero. The red star represents the experimentally measured Seebeck coefficient.

15
concentration which contributes to the reduction of the Seebeck coefficient. The cross-
plane Seebeck coefficient is larger than the in-plane Seebeck coefficient for the same
chemical potential. In the case of the Seebeck coefficient, there is no effect of vdW
interaction in the in-plane direction while there is a small but insignificant effect in the
cross-plane direction. Agarwal et al. reported experimentally measured room
temperature Seebeck coefficient of -960 µV/K at a carrier concentration of 1.78x10^{16} cm^{-}

3 [64]. The chemical potential that corresponds to this carrier concentration is 0.21 eV below the CBM. In Fig. 5(a), the experimental Seebeck coefficient is shown as a red star.

The calculated Seebeck coefficient of -1035 µV/K at room temperature at the chemical potential of 0.21 eV below the CBM is a reasonable estimate of the experimentally measured value. The inclusion of the combination of both the EPS rates and IIS rates in the Seebeck calculation does not have any effect on the Seebeck coefficients further confirming the insensitiveness of the Seebeck coefficient on the details of relaxation times.

**Conclusion **

In summary, we calculated the EPS rates of bulk MoSe2 using two full first principle- based codes, PERTURBO and EPW. The IIS rates are calculated using the Brooks-Herring method. The calculated EPS rates and IIS rates are then used to obtain the in-plane and the cross-plane electronic and thermoelectric properties of bulk MoSe2 at room temperature with and without including the vdW interaction using the BTE under the RTA. The calculated in-plane and cross-plane electron mobility with the inclusion of only

16
EPS rates at room temperature without and with incorporating the vdW interaction is
relatively insensitive to carrier concentration for a carrier concentration range of 10^{16} to
10^{18} cm^{-3}. The in-plane mobilities are not affected by the vdW interaction while the cross-
plane mobilities are reduced by 1.7 times thus confirming that the inclusion of vdW
interaction is important to accurately predict the cross-plane transport properties of
MoSe^{2}. The theoretically calculated in-plane electron mobilities are overestimated
compared to the experimental mobilities when only EPS rates are included. Similarly, for
the same carrier concentration range, the electrical conductivities calculated including
only the EPS rates under RTA shows a relatively higher value compared to the
experimentally measured values of single-crystal MoSe^{2 }in the in-plane direction. This is
consistent with the fact that electron transport is affected by other scattering mechanisms
such as IIS along with EPS. Therefore, we included both the EPS rates and IIS rates in the
transport calculation to obtain the in-plane and cross-plane transport properties. The
apparent agreement with no fitting parameters between the theoretically calculated and
experimentally measured in-plane electron mobilities and electrical conductivities
signifies that the transport in bulk MoSe2 at room temperature is dominated by the EPS
at low carrier concentration and the combination of EPS and IIS at high carrier
concentration. The Seebeck coefficientsare calculated by solving the linearizedelectron
BTE under the RTA with the aid of the first-principles EPS rates evaluated at different
Fermi Level positions. To compare the calculated Seebeck coefficient under RTA, the

17 Seebeck coefficients are again calculated using BTE under CRTA. The RTA and CRTA Seebeck coefficients show a good agreement indicating that the Seebeck coefficient is not sensitive to the details of the relaxation time. The inclusion of both the EPS rates and the IIS rates in the Seebeck calculation did not influence the Seebeck coefficients, further proving the insensitivity of the Seebeck coefficient to the specifics of relaxation times.

**Conflicts of interest **

There are no conflicts to declare.

**Acknowledgments **

This work is supported by NSF grant number 1653268. The authors acknowledge the
Rivanna High-Performance Computing system of the University of Virginia**. **

**References **

[1] *W. Liang, A. I. Hochbaum, M. Fardy, O. Rabin, M. Zhang, and P. Yang, Field-*
**Effect Modulation of Seebeck Coefficient in Single PbSe Nanowires, Nano Lett. 9, (2009). **

[2] *K. P. Pernstich, B. Rössner, and B. Batlogg, Field-Effect-Modulated Seebeck Coefficient *
**in Organic Semiconductors, Nat. Mater. 7, (2008). **

[3] M. S. Dresselhaus, G. Chen, M. Y. Tang, R. Yang, H. Lee, D. Wang, Z. Ren, J. P.

*Fleurial, and P. Gogna, New Directions for Low-Dimensional Thermoelectric Materials, *
**Adv. Mater. 19, (2007). **

18 [4] K. Biswas, J. He, I. D. Blum, C. I. Wu, T. P. Hogan, D. N. Seidman, V. P. Dravid,

*and M. G. Kanatzidis, High-Performance Bulk Thermoelectrics with All-Scale *
**Hierarchical Architectures, Nature 489, (2012). **

[5] *G. J. Snyder and E. S. Toberer, Complex Thermoelectric Materials, Nature Materials. *

[6] *M. Zebarjadi, K. Esfarjani, M. S. Dresselhaus, Z. F. Ren, and G. Chen, Perspectives *
* on Thermoelectrics: From Fundamentals to Device Applications, Energy Environ. Sci. 5, *
(2012).

[7] * F. J. DiSalvo, Thermoelectric Cooling and Power Generation, Science (80-. ). 285, 703 *
(1999).

[8] * B. C. Sales, THERMOELECTRIC MATERIALS: Smaller Is Cooler, Science (80-. ). 295, *
1248 (2002).

[9] * C. Wood, Materials for Thermoelectric Energy Conversion, Reports Prog. Phys. 51, *
459 (1988).

[10] L. E. Shelimova, O. G. Karpinskii, P. P. Konstantinov, E. S. Avilov, M. A. Kretova,
*and V. S. Zemskov, Crystal Structures and Thermoelectric Properties of Layered *

**Compounds in the ATe-Bi2Te3 (A = Ge, Sn, Pb) Systems, Inorg. Mater. 40, (2004). **

*[11] S. M. Kauzlarich, S. R. Brown, and G. Jeffrey Snyder, Zintl Phases for Thermoelectric *
*Devices, Dalt. Trans. 2099 (2007). *

19
*[12] J. A. Dolyniuk, B. Owens-Baird, J. Wang, J. V. Zaikina, and K. Kovnir, Clathrate *

*Thermoelectrics, Materials Science and Engineering R: Reports. *

*[13] K. Koumoto, I. Terasaki, and R. Funahashi, Complex Oxide Materials for Potential *
**Thermoelectric Applications, MRS Bull. 31, (2006). **

*[14] G. S. Nolas, D. T. Morelli, and T. M. Tritt, Skutterudites: A Phonon-Glass-Electron *
*Crystal Approach to Advanced Thermoelectric Energy Conversion Applications, Vol. 29 *
(1999).

*[15] M. Rull-Bravo, A. Moure, J. F. Fernández, and M. Martín-González, Skutterudites *
**as Thermoelectric Materials: Revisited, RSC Adv. 5, 41653 (2015). **

*[16] Rowe David michael, Introduction. In: CRC Handbook of Thermoelectrics (CRC Press, *
1995).

* [17] M. Zebarjadi, Electronic Cooling Using Thermoelectric Devices, Appl. Phys. Lett. 106, *
203506 (2015).

*[18] M. J. Adams, Verosky M., Zebarjadi M., and Heremans J. P., Active Peltier Coolers *
*Based on Correlated and Magnon-Drag Metals, Phys. Rev. Appl. (2019). *

*[19] M. J. Adams, M. Verosky, M. Zebarjadi, and J. P. Heremans, High Switching Ratio *
*Variable-Temperature Solid-State Thermal Switch Based on Thermoelectric Effects, Int. J. *

**Heat Mass Transf. 134, (2019). **

20
*[20] M. Markov and M. Zebarjadi, Thermoelectric Transport in Graphene and 2D Layered *

**Materials, Nanoscale Microscale Thermophys. Eng. 23, 117 (2019). **

[21] K. Hippalgaonkar, Y. Wang, Y. Ye, H. Zhu, Y. Wang, J. Moore, and X. Zhang,
*Record High Thermoelectric Powerfactor in Single and Few-Layer MoS$_2$, (2015). *

[22] J. Duan, X. Wang, X. Lai, G. Li, K. Watanabe, T. Taniguchi, M. Zebarjadi, and E. Y.

*Andrei, High Thermoelectricpower Factor in Graphene/HBN Devices, Proc. Natl. Acad. *

**Sci. 113, 14272 (2016). **

*[23] L. H. Brixner, Preparation and Properties of the Single Crystalline AB2-Type Selenides *
*and Tellurides of Niobium, Tantalum, Molybdenum and Tungsten, J. Inorg. Nucl. *

**Chem. 24, (1962). **

*[24] E. Revolinsky and D. Beerntsen, Electrical Properties of the MoTe2-WTe2 and MoSe *
**2-WSe2 Systems, J. Appl. Phys. 35, (1964). **

[25] A. Mavrokefalos, Q. Lin, M. Beekman, J. H. Seol, Y. J. Lee, H. Kong, M. T. Pettes,
*D. C. Johnson, and L. Shi, In-Plane Thermal and Thermoelectric Properties of Misfit-*
**Layered [(PbSe) 0.99] x (WSe2) x Superlattice Thin Films, Appl. Phys. Lett. 96, (2010). **

*[26] S. H. El‐Mahalawy and B. L. Evans, Temperature Dependence of the Electrical *

*Conductivity and Hall Coefficient in 2H‐MoS2, MoSe2, WSe2, and MoTe2, Phys. Status *
**Solidi 79, (1977). **

21 [27] C. Muratore, V. Varshney, J. J. Gengler, J. J. Hu, J. E. Bultman, T. M. Smith, P. J.

*Shamberger, B. Qiu, X. Ruan, A. K. Roy, and A. A. Voevodin, Cross-Plane Thermal *
**Properties of Transition Metal Dichalcogenides, Appl. Phys. Lett. 102, (2013). **

*[28] M. G. Rosul, M. S. Akhanda, and M. Zebarjadi, Thermionic Energy Conversion, in *
*Nanoscale Energy Transport (IOP Publishing, 2020), pp. 14-1-14–29. *

[29] M. G. Rosul, D. Lee, D. H. Olson, N. Liu, X. Wang, P. E. Hopkins, K. Lee, and M.

*Zebarjadi, Thermionic Transport across Gold-Graphene-WSe<inf>2</Inf> van Der *
**Waals Heterostructures, Sci. Adv. 5, (2019). **

*[30] X. Wang, M. Zebarjadi, and K. Esfarjani, High-Performance Solid-State Thermionic *
*Energy Conversion Based on 2D van Der Waals Heterostructures: A First-Principles *
**Study, Sci. Rep. 8, 9303 (2018). **

*[31] M. G. Rosul, X. Wang, K. Esfarjani, and M. Zebarjadi, Low-Resistance Contact in *
**MoSe2-Based Solid-State Thermionic Devices, Phys. Rev. B 105, 115412 (2022). **

*[32] A. Ziabari, M. Zebarjadi, D. Vashaee, and A. Shakouri, Nanoscale Solid-State *
**Cooling: A Review, Reports Prog. Phys. 79, (2016). **

*[33] Q. Li, Q. Hao, T. Zhu, M. Zebarjadi, and K. Takahashi, Nanostructured and *
**Heterostructured 2D Materials for Thermoelectrics, Eng. Sci. 13, 24 (2020). **

*[34] P. J. Lowell, G. C. O’Neil, J. M. Underwood, and J. N. Ullom, Macroscale *

22
**Refrigeration by Nanoscale Electron Transport, Appl. Phys. Lett. 102, 082601 (2013). **

*[35] G. Kioseoglou, A. T. Hanbicki, M. Currie, A. L. Friedman, and B. T. Jonker, Optical *
* Polarization and Intervalley Scattering in Single Layers of MoS2 and MoSe2, Sci. Rep. 6, *
25041 (2016).

*[36] W. S. Yun, S. W. Han, S. C. Hong, I. G. Kim, and J. D. Lee, Thickness and Strain *
*Effects on Electronic Structures of Transition Metal Dichalcogenides: 2H- MX2 *
**Semiconductors ( M = Mo, W; X = S, Se, Te), Phys. Rev. B 85, 033305 (2012). **

[37] S. Tongay, J. Zhou, C. Ataca, K. Lo, T. S. Matthews, J. Li, J. C. Grossman, and J.

*Wu, Thermally Driven Crossover from Indirect toward Direct Bandgap in 2D *
**Semiconductors: MoSe2 versus MoS2, Nano Lett. 12, (2012). **

*[38] R. E. Peierls, Quantum Theory of Solids (Oxford University Press, 2001). *

*[39] W. Kohn, Image of the Fermi Surface in the Vibration Spectrum of a Metal, Phys. Rev. *

**Lett. 2, 393 (1959). **

*[40] J. R. Schrieffer, Theory of Superconductivity (CRC Press, 2018). *

*[41] J. Zhou, B. Liao, and G. Chen, First-Principles Calculations of Thermal, Electrical, and *
* Thermoelectric Transport Properties of Semiconductors, Semicond. Sci. Technol. 31, *
043001 (2016).

*[42] S. Poncé, E. R. Margine, and F. Giustino, Towards Predictive Many-Body Calculations *

23
**of Phonon-Limited Carrier Mobilities in Semiconductors, Phys. Rev. B 97, (2018). **

*[43] S. Poncé, E. R. Margine, C. Verdi, and F. Giustino, EPW: Electron–Phonon Coupling, *
*Transport and Superconducting Properties Using Maximally Localized Wannier *

**Functions, Comput. Phys. Commun. 209, 116 (2016). **

*[44] L. A. Agapito and M. Bernardi, Ab Initio Electron-Phonon Interactions Using Atomic *
**Orbital Wave Functions, Phys. Rev. B 97, (2018). **

*[45] J.-J. Zhou, J. Park, I.-T. Lu, I. Maliyov, X. Tong, and M. Bernardi, Perturbo: A *
*Software Package for Ab Initio Electron–Phonon Interactions, Charge Transport and *
**Ultrafast Dynamics, Comput. Phys. Commun. 264, 107970 (2021). **

[46] G. Brunin, H. P. C. Miranda, M. Giantomassi, M. Royo, M. Stengel, M. J.

*Verstraete, X. Gonze, G. M. Rignanese, and G. Hautier, Phonon-Limited Electron *
*Mobility in Si, GaAs, and GaP with Exact Treatment of Dynamical Quadrupoles, Phys. *

**Rev. B 102, (2020). **

[47] A. A. Mostofi, J. R. Yates, Y. S. Lee, I. Souza, D. Vanderbilt, and N. Marzari,
*Wannier90: A Tool for Obtaining Maximally-Localised Wannier Functions, Comput. *

**Phys. Commun. 178, 685 (2008). **

*[48] D. Long and J. Myers, Ionized-Impurity Scattering Mobility of Electrons in Silicon, *
**Phys. Rev. 115, (1959). **

24 [49] P. Giannozzi, S. Baroni, N. Bonini, M. Calandra, R. Car, C. Cavazzoni, D. Ceresoli, G. L. Chiarotti, M. Cococcioni, I. Dabo, A. Dal Corso, S. de Gironcoli, S. Fabris, G.

Fratesi, R. Gebauer, U. Gerstmann, C. Gougoussis, A. Kokalj, M. Lazzeri, L.

Martin-Samos, N. Marzari, F. Mauri, R. Mazzarello, S. Paolini, A. Pasquarello, L.

Paulatto, C. Sbraccia, S. Scandolo, G. Sclauzero, A. P. Seitsonen, A. Smogunov, P.

*Umari, and R. M. Wentzcovitch, QUANTUM ESPRESSO: A Modular and Open-*
*Source Software Project for Quantum Simulations of Materials, J. Phys. Condens. *

**Matter 21, 395502 (2009). **

*[50] N. Troullier and J. L. Martins, Efficient Pseudopotentials for Plane-Wave Calculations, *
**Phys. Rev. B 43, 1993 (1991). **

*[51] J. P. Perdew, K. Burke, and M. Ernzerhof, Generalized Gradient Approximation Made *
**Simple, Phys. Rev. Lett. 77, 3865 (1996). **

*[52] M. Dion, H. Rydberg, E. Schröder, D. C. Langreth, and B. I. Lundqvist, Van Der *
**Waals Density Functional for General Geometries, Phys. Rev. Lett. 92, 246401 (2004). **

*[53] J. Klimeš, D. R. Bowler, and A. Michaelides, Van Der Waals Density Functionals *
**Applied to Solids, Phys. Rev. B 83, 195131 (2011). **

* [54] P. B. James and M. T. Lavik, The Crystal Structure of MoSe2, Acta Crystallogr. 16, *
(1963).

*[55] F. Giustino, M. L. Cohen, and S. G. Louie, Electron-Phonon Interaction Using *

25
**Wannier Functions, Phys. Rev. B 76, 165108 (2007). **

*[56] N. Marzari, A. A. Mostofi, J. R. Yates, I. Souza, and D. Vanderbilt, Maximally *
* Localized Wannier Functions: Theory and Applications, Rev. Mod. Phys. 84, 1419 *
(2012).

[57] T. Böker, R. Severin, A. Müller, C. Janowitz, R. Manzke, D. Voß, P. Krüger, A.

*Mazur, and J. Pollmann, Band Structure of MoS2, MoSe2, and α-MoTe2: Angle-*
*Resolved Photoelectron Spectroscopy and Ab Initio Calculations, Phys. Rev. B - *
**Condens. Matter Mater. Phys. 64, (2001). **

*[58] G. D. Mahan, Condensed Matter in a Nutshell (2019). *

[59] K.-K. Kam, Electrical Properties of WSe2, WS2, MoSe2, MoS2, and Their Use as Photoanodes in a Semiconductor Liquid Junction Solar Cell, Iowa State

University, 1982.

*[60] R. Fivaz and E. Mooser, Mobility of Charge Carriers in Semiconducting Layer *
**Structures, Phys. Rev. 163, (1967). **

*[61] F. Lévy, P. H. Schmid, and H. Berger, Electrical Properties of Layered MoSe2 Single *
**Crystals Doped with Nb and Re, Philos. Mag. 34, (1976). **

*[62] S. Y. Hu, C. H. Liang, K. K. Tiong, Y. C. Lee, and Y. S. Huang, Preparation and *
**Characterization of Large Niobium-Doped MoSe2 Single Crystals, J. Cryst. Growth 285, **

26 408 (2005).

*[63] G. K. H. Madsen and D. J. Singh, BoltzTraP. A Code for Calculating Band-Structure *
**Dependent Quantities, Comput. Phys. Commun. 175, 67 (2006). **

*[64] M. K. Agarwal, P. D. Patel, and S. K. Gupta, Effect of Doping MoSe2 Single Crystals *
**with Rhenium, J. Cryst. Growth 129, (1993). **

**Supplementary Information for Effect of electron-phonon ** **interaction on the room temperature thermoelectric properties **

**of bulk MoSe**

^{2}Md Golam Rosul^{1}, Mona Zebarjadi^{1,2,*}

1Department of Electrical and Computer Engineering, University of Virginia, Charlottesville, VA 22904, United States

2Department of Materials Science and Engineering, University of Virginia, Charlottesville, VA 22904, United States

*Corresponding author: mz6g@virginia.edu

**Quantum Espresso and Wannier band structure: **

The maximally localized Wannier function was used to interpolate the DFT band
structure. In the Wannier function, each Mo atom has dxy, dxz, dyz, dz^{2}, dx^{2}-y^{2} orbitals,
whereas each Se atom has px, py, pz orbitals, resulting in the wannierization of a total of
22 bands. Figure S1 shows the band structure calculated from DFT and by interpolation

27 using the maximally localized Wannier function. Both of these band structures show good agreement.

Figure S6. The band structure of MoSe^{2}. Results from DFT calculations (blue solid lines) and
Wannier interpolation (red solid lines) are overlaid.